1 GuideGrout Troubleshooting TABLE OF CONTENTSC ement Grout Symptom1-2 Grout discoloration3 Efflorescence4 Tile discoloration5 Grout cracking6 Grout with pinholes6 Powdery Grout in the jointsReady-to-Use (RTU) Grout Symptom7-8 Grout discoloration9 Efflorescence9 Tile discoloration10 Grout not curing11 Grout with pinholes11 Grout crackingEpoxy Grouts Symptom12-13 Grout discoloration13 Efflorescence14 Tile discoloration15 Grout with pinholes16 Grout cracking18-19 UltraCare Quick-reference guideOther20 Mapei Technical Institute1 SourcesSolutionsThe mixing water and/or the wash water used to clean had a high content of iron or other potable water, or use Mapei s UltraCareTM Grout Maximizer Grout conditions such as direct sun exposure, hot ambient or tile temperatures, or too much area being grouted at a time before initiating the cleanup process.
2 Protect tilework from direct sunlight during application, and always apply within the temperature ranges of the current Technical Data Sheet (TDS). Grout small areas of between 30 to 40 sq. ft. (2,79 to 3,72 m2) at a time, so that cleaning can begin before the Grout skins over and dries on the tile Grout color was not what was Mapei s UltraCare Grout RefreshTM Pre-Cleaner and UltraCare Grout Refresh to re-color and seal the joints at the same was added to the Grout powder instead of the powder being added to add the Grout powder to water for best results. This ensures proper dispersion of the Grout and produces a more uniform much water in the Grout will cause pigment washout, performance issues and a lighter-than-desired color.
3 Too little water can lead to performance issues like powdery Grout and shading (variable shades in the Grout color).Closely follow the mixing ratios found on the product label and Grout mix was not thoroughly recommended product mixing times on the product label and TDS. These mixing times will vary depending upon the type of cement Grout (sanded, unsanded, rapid-set). Grout was not allowed to slake (sit) after initial mixing. Follow the recommended slake time on the product label and slaking, remixing was performed too early, too late or not at slaking, always remix the Grout before beginning to use to tile-spacing lugs left in the Grout joints, variable depths of the joints caused a test area to determine the impact of the tile-spacing lugs on the Grout color.
4 Either use UltraCare Grout Release, or wet the tile surface with clean water. The varying density and porosity of the tile and natural stone caused the Grout to dry blotchy and to wet with UltraCare Grout Release, removing the temporary coating that is formed, or wet with joints were wiped excessively during the initial cleaning certain rough glazed or textured tile surfaces, there is a tendency to use excessive force to remove Grout haze. Use UltraCare Grout Release to minimize the need for excessive wiping during Grout powder was not dry-blended before adding water or admixture. Dry-blend the powder before adding water or admixture. This is especially important when you have more than one bag of product.
5 The bags could potentially be from different production runs or manufacturing plants, and have a slight color variation between Grout Symptom Grout discolorationA non-uniform, blotchy, shaded or dirty appearance of the Grout joint that can manifest from a number of different sourcesGrout discoloration2A non-uniform, blotchy, shaded or dirty appearance of the Grout joint that can manifest from a number of different sourcesSourcesSolutionsGrout cleaning was completed too early or too late after floating the Grout into the are differences in recommended wash (cleaning) times, depending upon what cement Grout is used for example, some grouts are rapid-set. Typically, cleaning is allowed between 15 to 30 minutes after grouting, or when there is no longer a transfer of Grout to your finger.
6 Check the product label and/or TDS to confirm the time before cleaning. Too much water was used during the cleaning process. Use a slightly moist sponge where water does not drip out. Follow recommended product application procedures on the product label and sealer was applied prematurely after 48 hours after grouting before applying a sealer. Follow recommended product application procedures on the product label and TDS. Refer to the UltraCare Quick-reference guide for sealer Grout s shelf life the product shelf life on the TDS. Dispose of the Grout if the shelf life has tile-setting material was not properly cured before that the tile-setting material is fully cured before was excessive tile-setting material in the Grout joint.
7 Remove dried residue from the Grout joints, ensuring that at least 2/3 of the joint depth is left available for were inconsistent Grout joint depths and gap widths. Use tile spacers to ensure proper color/appearance glazed on the tile edges caused the Grout to dry/cure at different times and lead to tile that has a uniform glaze coat on the concrete slab was not fully cured or had moisture-vapor the concrete s moisture levels with a calcium chloride test, or a relative humidity or moisture meter. Mapei moisture-reduction-barrier products can also be used. Grouting was done by different installers and under different environmental possible, use the same installer or group of installers and follow the same procedures.
8 In addition, try to maintain consistent environmental conditions. Different batch codes of Grout were used when more than one bag was the batch codes of the Grout bags. Select batch codes that are the same whenever possible this will minimize the potential for bag-to-bag color variation. Dry-blend bags of different lot numbers before adding water or admixtures to ensure maintenance cleaning of the Grout was performed too early after 72 hours before beginning routine maintenance cleaning of the color of the Grout became bleached out (washed out) some time after Mapei cement grouts are rated for both exterior and interior installations. As a result, bleached or washed-out Grout is not due to UV exposure.
9 Check for harsh chemicals (such as highly acidic cleaners) or other contaminants that could have caused this Grout Symptom Grout discoloration (continued)3 SSourcesSolutionsWater used in mixing and cleaning had a high content of iron and other potable water, or use Mapei s UltraCareTM Grout Maximizer Grout joints were wiped excessively during the initial cleaning certain rough glazed or textured tile surfaces, there is a tendency to use excessive force to remove Grout haze. Use UltraCare Grout Release to minimize the need for excessive wiping during much water or admixture was used to mix the the recommended product mixing procedures on the product label and Technical Data Sheet (TDS).Too much water was used during the cleaning a slightly moist sponge where water does not drip out.
10 Follow recommended product application procedures on the product label and temperature and humidity conditions occurred during installations should be completed in temperatures between 50 F and 95 F (10 C and 35 C). The tile-setting material was not properly cured before grouting, ensure that tile-setting materials are fully cured and that Grout areas are clean and moisture source was present in the existing underlying surface or surrounding area. Examples of moisture sources can include leaky plumbing, rain and damaged subfloors that allow moisture to Mapei s waterproofing or moisture-control products, and/or Mapei s rapid-setting products to set and Grout ( , UltraflexTM RS and Ultracolor Plus FA), in order to minimize the possibility for efflorescence and increase the opportunity to have consistent concrete slab was not cured or had moisture-vapor grouting on less than fully cured substrates.